A surface treatment technology that has developed rapidly recently is the electrostatic powder coating of architectural aluminum
profiles. Its characteristics are that the powder can be recycled, does not contain solvents, does not pollute the environment, is easy to realize automated manufacturing, is simple to use, and the coating can meet different weather resistance requirements. , The color is diversified. However, some defects often appear in the electrostatic powder spraying of aluminum profiles, resulting in poor appearance quality and performance of the product. The following are several common causes of coating defects and control measures: defect name: particle cause analysis: the substrate surface has burrs, aluminum chips and graphite marks, etc., and the pretreatment is not good; the pretreatment bath residue adheres to the surface of the profile and is washed with water Dirty is in place; the chromating material is placed for a long time before painting, and the surface is adsorbed by dust; the improper use of new burning tools causes the surface of the chromizing material to fall off; the powder and the recycled powder may contain impurities; the spraying site and the curing furnace are not Clean with suspended solids. Control measures: polish the surface of the blank or sandblast before the upper row to ensure that the pre-treatment is in place; regularly invert the tank, clean up the residue, and extend the pure water washing time; carefully blow the dust after the chromized material is discharged; spray a layer on the new burning rack Use after thin film coating; recycled powder should be used after sieving; the workshop implements 6S management, keeps the spraying site tidy, and regularly cleans the curing furnace. Defect name: Analysis of the cause of exposed bottom: poor coverage of powder coatings; complex cross-section structure of profiles may easily cause electrostatic shielding effects; improper hanging methods; poor sense of responsibility of spray booth workers, poor business ability, improper judgment of powder coating thickness; spray guns There is too much powder in the mouth and clogging; the moving speed of the spray gun is too fast or the chain speed is too fast; the understanding of the decorative surface of the profile is not clear. Control measures: strictly control the quality of powder coatings; manually add powder to the profile grooves and inner corners; adjust the profile hanging angle; improve the spray booth skills, and the spray booth workers try to measure the film thickness of the cured profile as soon as possible; clean the spray gun mouth regularly, Keep it unobstructed; adjust the moving speed of the spray gun and appropriately reduce the chain speed; understand the customer's spraying requirements and recognize the decorative surface of the profile. Defect name: Cause analysis of variegated color: When the spray booth worker changed the color and cleaned the spray booth, the cleaning was not thorough enough and the powder leaked and caused the variegated color; the powder (recycled powder) was not used in time to bake the board and the color was corrected; the environment around the spray booth was not clean. Control measures: When cleaning the spray booth, the spray booth workers must carefully clean up every detail, especially the spray gun powder pipes are thoroughly cleaned, and the large cyclone must be carefully blown out. After cleaning the spray booth, the baking sheet must be checked for variegation before painting; The recycled powder must be used after the baking sheet is confirmed to be qualified, and the surrounding area of u200bu200bthe spray room should be kept hygienic and clean at all times. Defect name: Analysis of the cause of uneven coating: improper suspension and arrangement of chromium materials; poor grounding of aluminum materials (individual racks have poor conductivity); uneven conveyor chain speed, or chain speed inconsistent with spray gun lifting speed, profile decoration The number of powder coverage on the surface is inconsistent; the powder output of the spray gun and powder atomization are improper; the compressed air pressure is unstable; the voltage of the high-electric static generator is unstable, and the static electricity is high. Control measures: strengthen the communication between the workers in the spray booth and the workers in the spray booth, do a good job in the selection of the corresponding hangers for the profile; check whether the hangers are conductive; the spray booth workers strengthen the function, and do the hanger density, chain speed and Coordination of lifting speed; control the ratio of powder pumping gas and powder feeding gas; strengthen equipment maintenance and maintain stable equipment operation.
have manifold custom aluminium extrusion effects, ranging from aluminum extrusion rail to aluminum window profile manufacturers.
If you already use custom aluminium extrusion elsewhere or want the ability to offer restricted chat access to certain individuals, custom aluminium extrusion aluminum extrusion rail offers you the most flexibility.
Latest technology and manufacturing equipment has improved the quality of custom aluminium extrusion.